A Study on Preparation and Property Evaluations of Composites Consisting of TPU/Triclosan Membranes and Tencel®/LMPET Nonwoven Fabrics

This study investigated eco-friendly antibacterial medical protective clothing via the nonwoven process and characteristic evaluations. Firstly, Tencel® fibers and low melting point polyester (LMPET) fibers (re-sliced and granulated from recycled PET bottles) were mixed at different ratios and then needle punched at diverse needle rolling depths. The influences of manufacturing parameters on the Tencel®/LMPET nonwoven fabrics were examined in terms of mechanical properties, water vapor transmission rate, and stiffness. Next, Tencel®/LMPET nonwoven fabrics were combined with thermoplastic polyurethane (TPU)/Triclosan antibacterial membranes that contained different contents of triclosan using melt processing technology. The resulting Tencel®/LMPET/TPU/Triclosan composites were characterized via different measurements; an optimal bursting strength of 86.86 N, an optimal horizontal tensile strength of 41.90 N, and an optimal stiffness along the MD and CD of 8.60 cm were recorded. Furthermore, the Tencel®/LMPET/TPU/Triclosan composites exhibited a distinct inhibition zone in the antibacterial measurement, and the hydrostatic pressure met the requirements of the EN 14126:2003 and GB 19082-200 disposable medical protective gear test standards.


Introduction
Tencel ® is the commercial title of Lyocell fibers that are cellulous fibers made by solvent spinning wood pulp using N-Methylmorpholine-N-oxide (NMMO) as the solvent. What Lyocell fibers employ is a cellulose fiber technique that does not require a chemical reaction [1]. When dissolved in NMMO, cellulose fibers do not break down. NMMO and polyhydroxy (-OH) jointly generate hydrogen bonds that can dissolve cellulose, during which the closed production process transforms cellulose into an electrospinning solution. The electrospinning solution becomes cellulose fibers with the help of the dry-jet wet spinning technology. Specifically, over 99% of NMMO can be recycled and reused without jeopardizing the environment, and it can naturally decompose, featuring a clean production thermoplastic plastics, e.g., injection, extruding, blow molding, and calendaring. In sum, TPU is particularly suitable for mass production of medium-and small-sized components.
Triclosan (TCS) is also known as Dichlorophenoxychlorophenol, with the chemical formula of C 12 H 7 Cl 3 O 2 , and is an efficient antibacterial agent and disinfectant. TCS appears resistant to biodegradation and is commonly a white or grayish crystal powder that emits a phenolic odor [26]. TCS is not water-soluble but easily dissolves in lye and organic solvents. TCS is a broad-spectrum antibacterial agent used against hepatitis B virus and staphylococcus. Everyday necessities grant an upper limit of triclosan of 0.3%; as such, it is commonly used in soap, toothpaste, and other chemical products [27,28]. The sterilization mechanism is that TCS adsorbs and then penetrates the cell walls of bacteria to interact with the lipids and proteins of the cytoplasm, thereby deteriorating the protein so as to kill the bacteria [29,30]. More TCS is added to medicated mouthwash when used in the treatment for Candida albicans, gingivitis, or mouth ulcers. Moreover, TCS can also be used as a plastic additive in the production of antibacterial trash bags and the like [31].
In this study, Tencel ® fibers and LMPET fibers were blended at different ratios (LMPET comes from recycled PET bottles), and the blends underwent the nonwoven process with different needle punch depths in order to form Tencel ® /LMPET nonwoven matrices. Next, a single-screw granulator was used to blend TPU pellets with diverse contents of TCS powders, forming TPU/Triclosan antibacterial membranes. Finally, Tencel ® /LMPET nonwoven matrices and TPU/Triclosan antibacterial membranes were combined to form eco-friendly antibacterial composites used in protective clothing. The composite nonwoven fabrics were tested for stiffness, water vapor transmission rate, scanning electron microscopic observation, antibacterial efficacy, and mechanical properties, thereby determining the optimal Tencel ® /LMPET/TPU/Triclosan antibacterial composites for protective clothing matrices. Taking advantage of the characteristics of the lower melting point of recycled PET bottles, LMPET was compounded with TPU/Triclosan by a hot pressing process without using adhesives. Whether LMPET or Tencel ® fibers are recycled or regenerated fibers, this research proposes such a concept in the hope that nonwoven fabrics used in medical protective clothing during the time of COVID-19 can be improved.

Preparation of Tencel ® /LMPET Nonwoven Fabrics
A porcupine opener was used to scatter Tencel ® and LMPET fibers separately, and the fibers were then mixed at blending ratios of 100/0, 90/10, 80/20, 70/30, and 60/40 wt% using a needle curtain. Afterwards, the Tencel ® /LMPET blends became fluffy due to the breaking-and-opening process by a cotton comber, a cylinder, and a doffer. The blended fibers were carded to form an aligned fiber mesh that was then transmitted to the top screen for lay-up formation. Passing through the shake screen of a reciprocating traverse forming machine, the aligned Tencel ® /LMPET fiber mesh was laminated over the bottom screen and then needle bonded via a needle punching machine, forming Tencel ® /LMPET nonwoven fabrics ( Figure 1). The needle punch parameters included a speed of 200 needle/min and a depth of 13 mm or 14 mm. Finally, the nonwoven fabrics and TPU/Triclosan underwent roller thermoforming at 160 • C at a speed of 7 rpm/min with a two-wheel embossing machine.
breaking-and-opening process by a cotton comber, a cylinder, and a doffer. The blended fibers were carded to form an aligned fiber mesh that was then transmitted to the top screen for lay-up formation. Passing through the shake screen of a reciprocating traverse forming machine, the aligned Tencel ® /LMPET fiber mesh was laminated over the bottom screen and then needle bonded via a needle punching machine, forming Tencel ® /LMPET nonwoven fabrics (Figure 1). The needle punch parameters included a speed of 200 needle/min and a depth of 13 mm or 14 mm. Finally, the nonwoven fabrics and TPU/Triclosan underwent roller thermoforming at 160 °C at a speed of 7 rpm/min with a two-wheel embossing machine.

Preparation of Tencel ® /LMPET/TPU Matrices for Antibacterial Membranes
In the production of TPU/Triclosan antibacterial membranes, the content of triclosan was 0, 0.01, 0.05, 0.1, and 0.2 wt% ( Figure 2). To start with, TPU pellets and triclosan powders were melt-blended at successive temperatures of 160, 170, and then 180 °C with a single-screw granulator, after which the blends were placed in a cooling bath to shape the TPU/Triclosan pellets. Finally, the pellets were dissolved in a TPU dissolution reaction tank and subsequently formed into TPU/Triclosan membranes with a thickness of 20 μm using a laminator. The Tencel ® /LMPET nonwoven fabric and TPU/Triclosan composite heat pressing temperature was 160 °C.

Characterizations
The air permeability of the fabrics was measured using an air permeability tester (TEXTEST FX 3300-IV, Libero Technology Co., Ltd., Guangzhou, China) as specified in the ASTM D737-04 test standard. The tearing strength of samples was measured using a universal strength testing machine (HT-2402, Hong Ta Co., Ltd., Taiwan, China) as specified in the CNS 12915 test standard; five samples of 150 mm × 75 mm for each

Preparation of Tencel ® /LMPET/TPU Matrices for Antibacterial Membranes
In the production of TPU/Triclosan antibacterial membranes, the content of triclosan was 0, 0.01, 0.05, 0.1, and 0.2 wt% ( Figure 2). To start with, TPU pellets and triclosan powders were melt-blended at successive temperatures of 160, 170, and then 180 • C with a single-screw granulator, after which the blends were placed in a cooling bath to shape the TPU/Triclosan pellets. Finally, the pellets were dissolved in a TPU dissolution reaction tank and subsequently formed into TPU/Triclosan membranes with a thickness of 20 µm using a laminator. The Tencel ® /LMPET nonwoven fabric and TPU/Triclosan composite heat pressing temperature was 160 • C.
breaking-and-opening process by a cotton comber, a cylinder, and a doffer. The blended fibers were carded to form an aligned fiber mesh that was then transmitted to the top screen for lay-up formation. Passing through the shake screen of a reciprocating traverse forming machine, the aligned Tencel ® /LMPET fiber mesh was laminated over the bottom screen and then needle bonded via a needle punching machine, forming Tencel ® /LMPET nonwoven fabrics ( Figure 1). The needle punch parameters included a speed of 200 needle/min and a depth of 13 mm or 14 mm. Finally, the nonwoven fabrics and TPU/Triclosan underwent roller thermoforming at 160 °C at a speed of 7 rpm/min with a two-wheel embossing machine.

Preparation of Tencel ® /LMPET/TPU Matrices for Antibacterial Membranes
In the production of TPU/Triclosan antibacterial membranes, the content of triclosan was 0, 0.01, 0.05, 0.1, and 0.2 wt% ( Figure 2). To start with, TPU pellets and triclosan powders were melt-blended at successive temperatures of 160, 170, and then 180 °C with a single-screw granulator, after which the blends were placed in a cooling bath to shape the TPU/Triclosan pellets. Finally, the pellets were dissolved in a TPU dissolution reaction tank and subsequently formed into TPU/Triclosan membranes with a thickness of 20 μm using a laminator. The Tencel ® /LMPET nonwoven fabric and TPU/Triclosan composite heat pressing temperature was 160 °C.

Characterizations
The air permeability of the fabrics was measured using an air permeability tester (TEXTEST FX 3300-IV, Libero Technology Co., Ltd., Guangzhou, China) as specified in the ASTM D737-04 test standard. The tearing strength of samples was measured using a universal strength testing machine (HT-2402, Hong Ta Co., Ltd., Taiwan, China) as specified in the CNS 12915 test standard; five samples of 150 mm × 75 mm for each

Characterizations
The air permeability of the fabrics was measured using an air permeability tester (TEXTEST FX 3300-IV, Libero Technology Co., Ltd., Guangzhou, China) as specified in the ASTM D737-04 test standard. The tearing strength of samples was measured using a universal strength testing machine (HT-2402, Hong Ta Co., Ltd., Taiwan, China) as specified in the CNS 12915 test standard; five samples of 150 mm × 75 mm for each specification were taken along the machine direction (MD) and the cross-machine direction (CD) for an average. The bursting strength of samples (130 mm × 130 mm) was measured at a test rate of 10 mm/min using a universal strength testing machine (HT-2402, Hong Ta Co., Ltd., Taiwan) as specified in the CNS 12915 test standard. The tensile strength of the samples (180 mm × 250 mm) was measured at a test rate of 305 ± 13 mm/min using a universal strength testing machine (HT-2402, Hong Ta Co., Ltd., Taiwan) as specified in the CNS 12915 test standard. The distance between clamps was 7.6 cm, and six samples for each specification were taken along the MD and CD. Afterwards, the average, standard deviation, and coefficient of variation were computed accordingly. The stiffness test was conducted using the cantilever method as specified in the CNS 12915 test standard, and the stiffness is presented in centimeters. The antibacterial measurement was conducted as specified in the JIS1902-2002 test standard with S. aureus (ATCC 25923) and E. coli (ATCC 25922). The presence and the size of the inhibition zone ( Figure 3) were observed and determined using Equation (1) [33]. The material structure, morphology, and element analysis of the fabricated materials were characterized by field-emission scanning electron microscopy (Hitachi SEM 4800, Tokyo, Japan).
where D means the diameter of the circular sample (i.e., 6-mm), and T shows whether the sample exhibits an inhibition zone. When (T − D) > 0 is true, it means that the sample has antibacterial efficacy.
specification were taken along the machine direction (MD) and the cross-machine direction (CD) for an average. The bursting strength of samples (130 mm × 130 mm) was measured at a test rate of 10 mm/min using a universal strength testing machine (HT-2402, Hong Ta Co., Ltd., Taiwan) as specified in the CNS 12915 test standard. The tensile strength of the samples (180 mm × 250 mm) was measured at a test rate of 305 ± 13 mm/min using a universal strength testing machine (HT-2402, Hong Ta Co., Ltd., Taiwan) as specified in the CNS 12915 test standard. The distance between clamps was 7.6 cm, and six samples for each specification were taken along the MD and CD. Afterwards, the average, standard deviation, and coefficient of variation were computed accordingly. The stiffness test was conducted using the cantilever method as specified in the CNS 12915 test standard, and the stiffness is presented in centimeters. The antibacterial measurement was conducted as specified in the JIS1902-2002 test standard with S. aureus (ATCC 25923) and E. coli (ATCC 25922). The presence and the size of the inhibition zone ( Figure 3) were observed and determined using Equation (1) [33]. The material structure, morphology, and element analysis of the fabricated materials were characterized by field-emission scanning electron microscopy (Hitachi SEM 4800, Tokyo, Japan).
where D means the diameter of the circular sample (i.e., 6-mm), and T shows whether the sample exhibits an inhibition zone. When (T − D) > 0 is true, it means that the sample has antibacterial efficacy.  Figure 4a,b show the tensile strength along the CD and MD of Tencel ® /LMPET nonwoven fabrics. The nonwoven process involves a needle punch that contributes mechanical reinforcement of the resulting nonwoven fabrics as the fibers are entangled and bonded in the fiber mesh. Based on the test results, a rise in the LPET fiber content had a positive influence on the tensile strength of Tencel ® /LMPET nonwoven fabrics. In particular, with a blending ratio of 60/40 wt%, Tencel ® /LMPET nonwoven fabrics exhibited a maximal tensile strength of 52.3 N, the result of which can be attributed to the presence of LMPET fibers. When hot-pressed, the sheath of LMPET fibers melted to form thermal bonding points; the more LMPET fibers, the more thermal bonding points, which in turn mechanically reinforces Tencel ® /LMPET nonwoven fabrics to a certain degree. On the other hand, Figure 4c,d indicate that Tencel ® /LMPET nonwoven fabrics showed a decreasing trend in stiffness when composed of more Tencel ® fibers. Without any special treatment, nonwoven fabrics consisting of LMPET fibers exhibit less comfort than those consisting of natural fibers. Hence, the presence of LMPET fibers has a negative influence on the air permeability and stiffness of Tencel ® /LMPET nonwoven fabrics. Contrastingly,  Figure 4a,b show the tensile strength along the CD and MD of Tencel ® /LMPET nonwoven fabrics. The nonwoven process involves a needle punch that contributes mechanical reinforcement of the resulting nonwoven fabrics as the fibers are entangled and bonded in the fiber mesh. Based on the test results, a rise in the LPET fiber content had a positive influence on the tensile strength of Tencel ® /LMPET nonwoven fabrics. In particular, with a blending ratio of 60/40 wt%, Tencel ® /LMPET nonwoven fabrics exhibited a maximal tensile strength of 52.3 N, the result of which can be attributed to the presence of LMPET fibers. When hot-pressed, the sheath of LMPET fibers melted to form thermal bonding points; the more LMPET fibers, the more thermal bonding points, which in turn mechanically reinforces Tencel ® /LMPET nonwoven fabrics to a certain degree. On the other hand, Figure 4c,d indicate that Tencel ® /LMPET nonwoven fabrics showed a decreasing trend in stiffness when composed of more Tencel ® fibers. Without any special treatment, nonwoven fabrics consisting of LMPET fibers exhibit less comfort than those consisting of natural fibers. Hence, the presence of LMPET fibers has a negative influence on the air permeability and stiffness of Tencel ® /LMPET nonwoven fabrics. Contrastingly, the subsequent lamination process and hot pressing also adversely affect the stiffness, which illustrates the uncomfortable texture of current medical protective clothing. In this study, the Tencel ® /LMPET ratio of 50/50 wt% was also employed, but the resulting nonwoven fabrics were composed of an excessive amount of LMPET fibers, which means that there were equally too many LMPET fibers forming too many thermal bonding points. Eventu-ally, the stiffness of the nonwoven fabrics was compromised too much, and the 50/50 group was thus excluded. the subsequent lamination process and hot pressing also adversely affect the stiffness, which illustrates the uncomfortable texture of current medical protective clothing. In this study, the Tencel ® /LMPET ratio of 50/50 wt% was also employed, but the resulting nonwoven fabrics were composed of an excessive amount of LMPET fibers, which means that there were equally too many LMPET fibers forming too many thermal bonding points. Eventually, the stiffness of the nonwoven fabrics was compromised too much, and the 50/50 group was thus excluded.

Air Permeability of Tencel ® /LMPET Nonwoven Fabrics
The air permeability of nonwoven fabrics is dependent on the size and quantity of the voids among fibers. The voids are correlated with the fiber traits, fabric structure, fabric thickness, and fabric finishing. The nonwoven air permeability mechanism means that, being isolated by the fabric, the air with a higher pressure passes through the fabric from one specified side to the opposite side. Figure 5 compares the air permeability of Tencel ® /LMPET nonwoven fabrics when they were produced using a needle punch depth of 13 mm and 14 mm, and the air permeability fell in the range of 144.75~175 cm 3 /s/cm 2 . Tencel ® fibers have a smooth and sleek surface and feature excellent moisture repelling, air permeability, and cooling properties. Hence, Tencel ® /LMPET nonwoven fabrics showed a higher air permeability when consisting of more Tencel ® fibers.

Air Permeability of Tencel ® /LMPET Nonwoven Fabrics
The air permeability of nonwoven fabrics is dependent on the size and quantity of the voids among fibers. The voids are correlated with the fiber traits, fabric structure, fabric thickness, and fabric finishing. The nonwoven air permeability mechanism means that, being isolated by the fabric, the air with a higher pressure passes through the fabric from one specified side to the opposite side. Figure 5 compares the air permeability of Tencel ® /LMPET nonwoven fabrics when they were produced using a needle punch depth of 13 mm and 14 mm, and the air permeability fell in the range of 144.75~175 cm 3 /s/cm 2 . Tencel ® fibers have a smooth and sleek surface and feature excellent moisture repelling, air permeability, and cooling properties. Hence, Tencel ® /LMPET nonwoven fabrics showed a higher air permeability when consisting of more Tencel ® fibers. the subsequent lamination process and hot pressing also adversely affect the stiffness, which illustrates the uncomfortable texture of current medical protective clothing. In this study, the Tencel ® /LMPET ratio of 50/50 wt% was also employed, but the resulting nonwoven fabrics were composed of an excessive amount of LMPET fibers, which means that there were equally too many LMPET fibers forming too many thermal bonding points. Eventually, the stiffness of the nonwoven fabrics was compromised too much, and the 50/50 group was thus excluded.

Air Permeability of Tencel ® /LMPET Nonwoven Fabrics
The air permeability of nonwoven fabrics is dependent on the size and quantity of the voids among fibers. The voids are correlated with the fiber traits, fabric structure, fabric thickness, and fabric finishing. The nonwoven air permeability mechanism means that, being isolated by the fabric, the air with a higher pressure passes through the fabric from one specified side to the opposite side. Figure 5 compares the air permeability of Tencel ® /LMPET nonwoven fabrics when they were produced using a needle punch depth of 13 mm and 14 mm, and the air permeability fell in the range of 144.75~175 cm 3 /s/cm 2 . Tencel ® fibers have a smooth and sleek surface and feature excellent moisture repelling, air permeability, and cooling properties. Hence, Tencel ® /LMPET nonwoven fabrics showed a higher air permeability when consisting of more Tencel ® fibers.  Moreover, a higher needle punch depth also showed a negative influence on the air permeability of the Tencel ® /LMPET nonwoven fabrics because the fibers were entangled to a greater extent when they were needle punched by barbed fibers at a greater depth. By comparison, the 60/40 blending ratio provided nonwoven fabrics with a marginally lower strength than the 100/0 blending ratio, yet the 60/40 group still outperformed the other groups with different blending ratios in terms of mechanical properties. As a result, the optimal Tencel ® /LMPET nonwoven fabrics were produced with a blending ratio of 60/40 wt% and a needle punch depth of 14 mm, and this specified group of nonwoven fabrics was combined with the antibacterial TPU/triclosan membranes afterwards. Figure 6a shows that the Tencel ® /LMPET/TPU/Triclosan composites had an optimal bursting strength of 83 ± 7 N, while Figure 6b shows the test results of water vapor transmission that indicates how efficiently the composites release moisture and sweat vapor to keep wearers comfortable and dry without locking in heat around the skin. Based on EN 14126:2003 and GB 19082-2003 (specifications for verification of disposable one-piece medical protective clothing), the water vapor transmission of Tencel ® /LMPET/TPU/Triclosan composites was measured and found to be better than the requirement of the test standard (1500 g/m 2 /24 h) [34][35][36][37]. Furthermore, Figure 6c shows that the tensile strength along the MD was 53.2 N for the composites without triclosan. When the composites were composed of a greater amount of triclosan, the tensile strength showed a declining trend. With 0.2 wt% of triclosan, the tensile strength along the CD of the composites was 33.5 N. Figure 6d compares the influence of the MD and the CD on the tensile strength of the Tencel ® /LMPET/TPU/Triclosan composites. The tensile strength along the MD was lower and was only 20.1 N. Similarly, with a rise in the triclosan content, the tensile strength of the composites also decreased. Due to the presence of triclosan, the membranes contained more impurities, which in turn jeopardized the tensile strength.

Bursting Strength of Tencel ® /LMPET/TPU/Triclosan Composites
Moreover, a higher needle punch depth also showed a negative influence on the air permeability of the Tencel ® /LMPET nonwoven fabrics because the fibers were entangled to a greater extent when they were needle punched by barbed fibers at a greater depth. By comparison, the 60/40 blending ratio provided nonwoven fabrics with a marginally lower strength than the 100/0 blending ratio, yet the 60/40 group still outperformed the other groups with different blending ratios in terms of mechanical properties. As a result, the optimal Tencel ® /LMPET nonwoven fabrics were produced with a blending ratio of 60/40 wt% and a needle punch depth of 14 mm, and this specified group of nonwoven fabrics was combined with the antibacterial TPU/triclosan membranes afterwards. Figure 6a shows that the Tencel ® /LMPET/TPU/Triclosan composites had an optimal bursting strength of 83 ± 7 N, while Figure 6b shows the test results of water vapor transmission that indicates how efficiently the composites release moisture and sweat vapor to keep wearers comfortable and dry without locking in heat around the skin. Based on EN 14126:2003 and GB 19082-2003 (specifications for verification of disposable onepiece medical protective clothing), the water vapor transmission of Tencel ® /LMPET/TPU/Triclosan composites was measured and found to be better than the requirement of the test standard (1500 g/m 2 /24 h) [34][35][36][37]. Furthermore, Figure 6c shows that the tensile strength along the MD was 53.2 N for the composites without triclosan. When the composites were composed of a greater amount of triclosan, the tensile strength showed a declining trend. With 0.2 wt% of triclosan, the tensile strength along the CD of the composites was 33.5 N. Figure 6d compares the influence of the MD and the CD on the tensile strength of the Tencel ® /LMPET/TPU/Triclosan composites. The tensile strength along the MD was lower and was only 20.1 N. Similarly, with a rise in the triclosan content, the tensile strength of the composites also decreased. Due to the presence of triclosan, the membranes contained more impurities, which in turn jeopardized the tensile strength.   Figure 7b shows that the TPU/Triclosan antibacterial membranes had a   Figure 7b shows that the TPU/Triclosan antibacterial membranes had a thickness of 20 ± 0.12 µm, which changed marginally after undergoing the lamination process. Figure 7c shows the SEM image of fractured composites after the bursting strength test. The bursting strength performance of the TPU/Triclosan antibacterial membranes correlated with the presence of triclosan at diverse contents except for 0.1%. Consecutive cracking is absent in the resulting TPU/Triclosan antibacterial membranes that consist of 0.1 wt% of triclosan.

SEM Observation of Tencel ® /LMPET/TPU/Triclosan Composites
thickness of 20 ± 0.12 μm, which changed marginally after undergoing the lamination process. Figure 7c shows the SEM image of fractured composites after the bursting strength test. The bursting strength performance of the TPU/Triclosan antibacterial membranes correlated with the presence of triclosan at diverse contents except for 0.1%. Consecutive cracking is absent in the resulting TPU/Triclosan antibacterial membranes that consist of 0.1 wt% of triclosan.

Antibacterial Efficacy of Tencel ® /LMPET/TPU/Triclosan Composites
In this study, triclosan was used as an antibacterial agent, and S. aureus (Grampositive bacteria) and E. coli (Gram-negative bacteria) were used in the qualitative antimicrobial testing. The antibacterial measurement results are shown in Table 1. Figure  8 indicates that the antibacterial efficacy was proportional to the triclosan content. Specifically, the inhibition zone against S. aureus was 5.9 ± 0.3 mm when the antibacterial membranes consisted of 0.1 wt% of triclosan, showing a stabilized trend. In Figure 8b, the antibacterial membranes exhibit greater antibacterial efficacy against S. aureus than E. coli. Triclosan and silver ions share the same antibacterial mechanism, and the surface of both items carries positive charges that can draw the negative charges of the bacteria, thereby damaging the cell walls of the bacteria as well as preventing the fatty acids from synthesizing. Subsequently, the growth and function of biological cells are hampered, which eventually causes the death of the bacteria. In addition, the most significant difference between Gram-positive bacteria and Gram-negative bacteria is the thickness of the cell walls, which means that S. aureus possesses a lower thickness and is vulnerable to the penetration of triclosan. Hence, TPU/Triclosan membranes can prevent the synthesis of fatty acids inside the cytoplasm, attaining antibacterial efficacy or even achieving a sterilization effect.

Antibacterial Efficacy of Tencel ® /LMPET/TPU/Triclosan Composites
In this study, triclosan was used as an antibacterial agent, and S. aureus (Gram-positive bacteria) and E. coli (Gram-negative bacteria) were used in the qualitative antimicrobial testing. The antibacterial measurement results are shown in Table 1. Figure 8 indicates that the antibacterial efficacy was proportional to the triclosan content. Specifically, the inhibition zone against S. aureus was 5.9 ± 0.3 mm when the antibacterial membranes consisted of 0.1 wt% of triclosan, showing a stabilized trend. In Figure 8b, the antibacterial membranes exhibit greater antibacterial efficacy against S. aureus than E. coli. Triclosan and silver ions share the same antibacterial mechanism, and the surface of both items carries positive charges that can draw the negative charges of the bacteria, thereby damaging the cell walls of the bacteria as well as preventing the fatty acids from synthesizing. Subsequently, the growth and function of biological cells are hampered, which eventually causes the death of the bacteria. In addition, the most significant difference between Gram-positive bacteria and Gram-negative bacteria is the thickness of the cell walls, which means that S. aureus possesses a lower thickness and is vulnerable to the penetration of triclosan. Hence, TPU/Triclosan membranes can prevent the synthesis of fatty acids inside the cytoplasm, attaining antibacterial efficacy or even achieving a sterilization effect. . Samples with a water pressure resistance as high as 140 cm/H 2 O meet the requirements of the test standards. Regard-less of the triclosan content, all of the Tencel ® /LMPET/TPU/Triclosan composites are qualified to provide a water resistance of 537-549 cm/H 2 O, since TPU molecular chains contain smaller-sized molecular arrangement holes and therefore possess the waterproof feature. At room temperature, TPU membranes have waterproof properties without being jeopardized by water or moisture and provide the composites with an advantage that they can be used in a high-humidity environments or in contact with water. Regarding EN 14126:2003 andGB 19082-2003, it is stipulated that the strength of materials in key parts of protective clothing is not less than 45 N, and the data in this study are all greater than 45 N. The standard stipulates that the hydrostatic pressure should not be lower than 1.67 kPa (17 cm/H 2 O). This study found a value of 537-549 cm/H 2 O, which depends on the superior performance of TPU.   Figure 9a shows the stiffness of Tencel ® /LMPET/TPU/Triclosan composites in relation to the triclosan content. During the combination, the seepage of TPU/Triclosan reduced the friction level of the fluffy Tencel ® /LMPET nonwoven fabrics, improving the stiffness concurrently. The seepage also expelled the air in the voids of the nonwoven fabrics, resulting in a greater adhesion level between the Tencel ® /LMPET nonwoven fabrics and the TPU/Triclosan antibacterial membranes. Regardless of whether it was along the MD or CD, the stiffness of the Tencel ® /LMPET/TPU/Triclosan composites improved. Figure 9b shows the water resistance measurement (JISL 1092 B) of the Tencel ® /LMPET/TPU/Triclosan composites as specified in EN 14126:2003 and GB 19082-2003 (specifications for verification of disposable one-piece medical protective clothing) [37]. Samples with a water pressure resistance as high as 140 cm/H2O meet the requirements of the test standards. Regardless of the triclosan content, all of the Tencel ® /LMPET/TPU/Triclosan composites are qualified to provide a water resistance of 537-549 cm/H2O, since TPU molecular chains contain smaller-sized molecular arrangement holes and therefore possess the waterproof feature. At room temperature, TPU membranes have waterproof properties without being jeopardized by water or moisture and provide the composites with an advantage that they can be used in a highhumidity environments or in contact with water. Regarding EN 14126:2003 and GB 19082-

Conclusions
Overall, Tencel ® /LMPET nonwoven fabrics were optimal when the blending ratio was 60/40 wt% and the needle punch depth was 14 mm. Comparing to a needle punch depth of 13 mm, the needle punch depth of 14 mm improved the tearing strength, bursting strength, and tensile strength by 65%, 27%, and 11%, respectively. In addition, a needle punch depth of 15 mm broke the needles, whereas a needle punch depth of 12 mm failed to entangle the fibers effectively; thus, the optimal needle punch depth is 14 mm. As for

Conclusions
Overall, Tencel ® /LMPET nonwoven fabrics were optimal when the blending ratio was 60/40 wt% and the needle punch depth was 14 mm. Comparing to a needle punch depth of 13 mm, the needle punch depth of 14 mm improved the tearing strength, bursting strength, and tensile strength by 65%, 27%, and 11%, respectively. In addition, a needle punch depth of 15 mm broke the needles, whereas a needle punch depth of 12 mm failed to entangle the fibers effectively; thus, the optimal needle punch depth is 14 mm. As for TPU/Triclosan antibacterial membranes with a thickness of 20 µm containing triclosan (0, 0.01, 0.05, 0.1, and 0.2 wt%), only 0.1 wt% of triclosan helped to generate a distinctive inhibition zone and provided the membranes with antibacterial efficacy; however, 0.2 wt% of triclosan showed an adverse effect on the mechanical properties. Furthermore, with a trivial amount of triclosan, TPU membranes acquired antibacterial efficacy while improving diverse properties, which suggests that the incorporation of triclosan is one of the valuable additive parameters. Compared with the standard as shown in Table 2 below, the tensile strength in this study needs to be improved in the CD direction, and the moisture permeability also needs to be improved. Tencel ® has lower strength than polyester, but better comfort, and LMPET uses recycled PET bottle slices, meaning the strength will be decreased. All other indicators meet the standard requirements. One of the reasons for the lack of strength is that no adhesive was used. The low melting point of LMPET was used for bonding with nonwoven fabrics through hot-pressed bonding points.